MOLD SAND, SAND ADDITIVES & SAND PROPERTIES Collection and Selection by Dr. Mehdi Divandari IUST Casting Cast g1 Flow Chart of a Metal Casting System Sand Casting of Metals Mold Materials Topics covered: Molding sand Constituents of molding sand Property requirements of molding sand Testing of sand properties 1 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Mold Material The mold material is the one out of which the mold is made. The mold material should be such that casting should be able to retain its shape till the molten metal has solidified. Types of molds: Permanent molds: They are made up of ferrous metals and alloys (Steel, Grey CI, etc.). Temporary refractory molds: They are made of refractory sands and resins Molds made of wax, plastic, Plaster of Paris , carbon, ceramics are also employed. 2 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Mold Material Permanent molds They are employed for casting low melting point materials Temporary refractory molds Since they are made of refractory sands, the temporary refractory molds employed for casting high melting point materials They are costly. They are cheaper. They are employed to produce objects They are employed to produce objects bigger smaller in size. in size. They produce casting with better surface finish, quality and dimensional accuracy. 3 The surface finish, quality and dimensional accuracy of the casting temporary molds is poor. Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) produced by Properties of Molding Material Flowability – It is ability of molding sand to get compacted to a uniform density. Flowability assists molding sand to flow and pack all around the pattern and take up the required shape. The sand mold should response to different molding processes. Flowability increases as the clay and water content increases. Green Strength The molding sand that contains moisture is termed as green sand. The strength of the sand in green or moist state is termed as green strength. A mold with adequate green strength will be able to retain its shape and will not distort or collapse. The green sand particles have the ability to cling to each other to impart sufficient strength to the mold. Collapsibility It is property due to which the sand mold automatically gets collapsed after casting solidifies. The molding sand should also have collapsibility so that during the contraction of the casting it does not provide any resistance, which may result in the cracks in the casting. 4 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Properties of Molding Material Dry Strength It is the strength of the molding sand in dry conditions. When the molten metal is poured in the mold, the sand around the mold cavity is quickly converted into dry sand as the moisture in the sand evaporates due to the heat of the molten metal. At this stage the molding sand must posses the sufficient strength to retain the exact shape of the mold cavity and at the same time it must be able to withstand the metallostatic pressure of the liquid material. Dry sand strength is related to grain size, binder and water content. Permeability During pouring and subsequent solidification of a casting, a large amount of gases and steam is generated. These gases are those that have been absorbed by the metal during melting, air absorbed from the atmosphere and the steam generated by the molding and core sand. The binder, additives, etc. present in the molding sand also produce steam and other gases. If these gases are not allowed to escape from the mold, they would be entrapped inside the casting and cause casting defects. To overcome this problem the molding material must be porous or permeable to provide path for the escape of gases. Proper venting of the mold also helps in escaping the gases that are generated inside the mold cavity. Sand with Coarse grains exhibit more permeability. In absence of permeability the defects like surface blows, gas holes, etc. may be experienced. 5 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Properties of Molding Material Hot Strength It is strength of the sand above 212oF. As soon as the moisture is eliminated, the sand would reach at a high temperature when the metal in the mold is still in liquid state. The strength of the sand that is required to hold the shape of the cavity is called hot strength. In absence of hot strength the mold may enlarge, break, erode or get cracked. Durability – The molding sand should possess the capacity to withstand repeated cycles of heating and cooling during casting process Molding sand should be chemically immune to molten metals. Should be reusable. It should be easy to prepare and control. 6 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Properties of Molding Material Refractoriness It is the ability of the molding material to withstand the temperature of the liquid metal to be poured so that it does not get cracked, fused with the metal or experience any major physical change. Refractoriness is essential while casting high melting point materials. The refractoriness of the silica sand is highest. Fineness – Finer sand molds resists metal penetration and produces smooth casting surface. Fineness and permeability are in conflict with each other and hence they must be balanced for optimum results. Bench Life – It is ability of the molding sand to retain its properties during storage. Besides these specific properties the molding material should be cheap, reusable, coefficient of expansion, durability and should have good thermal conductivity. 7 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Molding Sands: Sources, Types, Ingredients Sources: Types: Ingredients: River beds Natural sands Refractory sand grains Sea Synthetic sands Binders Lakes Loam sands Water (moisture) Desert Additives 8 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Natural Sands It can be used as soon as received from source. It contains binding material (5-20%), water (5-8%) and considerable amount of organic matter. It can maintain moisture contain for long time. The finishing obtained on natural sand molds is good. It is cheaper compared to other sands. It has lesser refractoriness. It is employed for casting CI and non-ferrous metals. Molds made of natural sand can be easily repaired. When mixed with Bentonite, the properties of the sand gets improved and it gets properties like Synthetic sand. 9 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Synthetic Sands A synthetic sand consists of natural sand with or without clay, binder and moisture. The organic matter is not present in synthetic sand. Synthetic sand is a formulated sand, formulation is done to impart certain desired properties not possessed by natural sand. Possesses good refractoriness, high permeability, uniform grain size as compared to natural sand. It is more suitable for mass production and mechanized foundries. 10 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Loam Sands It contains much more clay (50% or more) as compared to ordinary sand. The ingredients of Loam sand may be fine sand, clay, finely ground refractories, graphite and fibrous reinforcement. 11 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Refractory Sands 1. Silica sand 2. Magnite 3. Zircon 4. Dolomite 5. Olivine 6. Silimanite 7. Graphite / Carbon 12 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Properties of Refractory Sands They maintain their shape and other characteristics at high temperature. When packed to produce the mold cavity, they remain sufficiently porous or permeable to give out gases produced during solidification of molten material. They can be molded into intricate shapes. They are chemically immune to molten metals. They can be used repeatedly to make molds. They are inexpensive. They can be made available without much difficulty. 13 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Molding Sand Composition Base Sand Silica sand is most commonly used base sand. Other base sands that are also used for making mold are zircon sand, Chromite sand and olivine sand. Silica sand is cheapest among all types of base sand and it is easily available. Binder Binders are of many types such as, Clay binders, Organic binders and Inorganic binders Clay binders are most commonly used binding agents mixed with the molding sands to provide the strength. The most popular clay types are: Kaolinite or fire clay (Al2O3 2SiO2 2H2O) and Bentonite (Al2O3 4SiO2 nH2O) Bentonite can absorb more water than fire clay which increases its bonding power. Water (Moisture) Clay acquires its bonding action only in the presence of the required amount of moisture. When water is added to clay, it penetrates the mixture and forms a microfilm, which coats the surface of each flake of the clay. The amount of water used should be properly controlled. This is because a part of the water, which coats the surface of the clay flakes, helps in bonding, while the remainder helps in improving the plasticity. 14 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Molding Sand Composition Typical Composition of Molding Sand 15 Molding Sand Constituent Weight (%) Silica sand 92 Clay (Sodium Bentonite) 8 Water 4 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Grain Size The grain shape and size of molding sand defines the total surface area of grains contained in unit mass. Total surface area is known as Specific Surface. Specific surface gives rough idea of amount of binder needed to coat the grains of molding sand. 16 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) Grain Size The grain size and distribution influences many sand properties such as permeability, flowability, refractoriness, surface fineness and strength. The finer the sand grains, the finer is the molding sand as whole. Fine grain sands give good surface finish but possess low permeability. For same clay content, the green strength is higher in case of fine sands as compared to coarse sands. Coarse and uniformly graded sand imparts high permeability, good refractoriness and high flowability. Normally the foundry sand possess the grain size between 0.1 to 1.0 mm The fine grained sands are used to make intricate and small size castings. Coarse grained sands are used to make large castings. 17 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) SAND Casting Sands • • • • • Silica Sands Zircon Olivine Chromite Aluminum Silicates Silica Sands • Most green sand molds consist of silica sands bonded with a bentonite‐water mixture. (The term green means that the mold, which is tempered with water, is not dried or baked.) The composition, size, size distribution, purity, and shape of the sand are important to the success of the mold making operation. • Sands are sometimes referred to as natural or synthetic. • Natural or Synthetic • Natural sands contain enough naturally occurring clays that they can be mixed with water and used for sand molding. • Synthetic sands have been washed to remove clay and other impurities, carefully screened and classified to give a desired size distribution, and then reblended with clays and other materials to produce an optimized sand for the casting being produced. • Because of the demands of modern high‐pressure molding machines and the necessity to exercise close control over every aspect of casting production, most foundries use only synthetic sands. Composition • Foundry sands are composed almost entirely of silica (SiO2) in the form of quartz. Some impurities may be present, such as ilmenite (FeO‐TiO2), magnetite (Fe3O4), or olivine, which is composed of magnesium and ferrous orthosilicate [(Mg,Fe) SiO4]. Silica sand is used primarily because it is readily available and inexpensive. • Quartz undergoes a series of crystallographic transitions as it is heated. The first, at 573 °C, is accompanied by expansion, which can cause mold spalling. Above 870 °C, quartz transforms to tridymite, and the sand may actually contract upon heating. At still higher temperatures (> 1470 °C), tridymite transforms to cristobalite. Shape and Distribution of Sand Grains • The size, size distribution, and shape of the sand grains are important in controlling the quality of the mold. Most mold aggregates are mixtures of new sand and reclaimed sand, which contain not only reclaimed molding sand but also core sands. In determining the size, shape, and distribution of the sand grains, it is important to realize that the grain shape contributes to the amount of sand surface area and that the grain size distribution controls the permeability of the mold. • As the sand surface area increases, the amount of bonding material (normally clay and water) must increase if the sand is to be properly bonded. Thus, a change in surface area, perhaps due to a change in sand shape or the percentage of core sand being reclaimed, will result in a corresponding change in the amount of bond required. • Rounded grains have a low surface‐area‐to‐volume ratio and are therefore preferred for making cores because they require the least amount of binder. However, when they are recycled into the molding sand system, their shape can be a disadvantage if the molding system normally uses a high percentage of clay and water to facilitate rapid, automatic molding. This is because rounded grains require less binder than the rest of the system sand. • Angular sands have the greatest surface area (except for sands that fracture easily and produce a large percentage of small grains and fines) and therefore require more mulling, bond, and moisture. The angularity of a sand increases with use because the sand is broken down by thermal and mechanical shock. • The porosity of the mold controls its permeability, which is the ability of the mold to allow gases generated during pouring to escape through the mold. The highest porosity will result from grains that are all approximately the same size. • As the size distribution broadens, there are more grains that are small enough to fill the spaces between large grains. As grains break down through repeated recycling, there are more and more of the smaller grains, and the porosity of the mold decreases. • However, if the porosity of the mold is too great, metal may penetrate the sand grains and cause a burn‐in defect. • Therefore, it is necessary to balance the base sand distribution and continue to screen the sand and use dust collectors during recycling to remove fines and to determine the proper bond addition. • Most foundries in the United States use the American Foundrymens' Society (AFS) grain fineness number as a general indication of sand fineness. The AFS grain fineness number of sand is approximately the number of openings per inch of a given sieve that would just pass the sample if its grains were of uniform size, that is, the weighted average of the sizes of grains in the sample. It is approximately proportional to the surface area per unit weight of sand exclusive of clay. Zircon • Zircon is zirconium silicate (ZrSiO4). It is highly refractory and possesses excellent foundry characteristics. Its primary advantages are a very low thermal expansion, high thermal conductivity and bulk density (which gives it a chilling rate about four times that of quartz), and very low reactivity with molten metal. Zircon requires less binder than other sands because its grains are rounded. The very high dimensional and thermal stabilities exhibited by zircon are the reasons it is widely used in steel foundries and investment foundries making high‐temperature alloy components. Olivine • Olivine minerals (so called because of their characteristic green color) are a solid solution of forsterite (Mg2SiO4) and fayalite (Fe2SiO4). Their physical properties vary with their chemical compositions; therefore, the composition of the olivine used must be specified to control the reproducibility of the sand mixture. Care must be taken to calcine the olivine sand before use to decompose the serpentine content, which contains water . • The specific heat of olivine is similar to that of silica, but its thermal expansion is far less. Therefore, olivine is used for steel casting to control mold dimensions. Olivine is somewhat less durable than silica , and it is an angular sand. Chromite • Chromite (FeCr2O4), a black, angular sand, is highly refractory and chemically unreactive, and it has good thermal stability and excellent chilling properties. However, it has twice the thermal expansion of zircon sand, and it often contains hydrous impurities that cause pinholing and gas defects in castings. It is necessary to specify the calcium oxide (CaO) and silicon dioxide (SiO2) limits in chromite sand to avoid sintering reactions and reactions with molten metal that cause burn‐in. Aluminum Silicates • Aluminum silicate (Al2SiO5) occurs in three common forms: kyanite, sillimanite, and andalusite. All break down at high temperatures to form mullite and silica . Therefore, aluminum silicates for foundry use are produced by calcining these minerals. Depending on the sintering cycle, the silica may be present as cristobalite or as amorphous silica. The grains are highly angular. These materials have high refractoriness, low thermal expansion, and high resistance to thermal shock. They are widely used in precision investment foundries, often in combination with zircon. Bulk density =The mass of powdered or granulated solid material per unit of volume SAND ADDITIVES Water • Water • H0 2 SAND ADDITIVES Clays • • • • • Clays Bentonite, Southern (Ca‐Bentonite) Bentonite, Western (Na‐Bentonite) Fireclay Kaolin Clay • The most common clays used in bonding green sand molds are bentonites, which are forms of montmorillonite or hydrated aluminum silicate. Montmorillonite is built up of alternating tetrahedra of silicon atoms surrounded by oxygen atoms, and aluminum atoms surrounded by oxygen atoms, as shown in Fig. 1. This is a layered structure, and it produces clay particles that are flat plates. Water is adsorbed on the surfaces of these plates, and this causes bentonite to expand in the presence of water and to contract when dried. SAND ADDITIVES Clays SAND ADDITIVES Clays SAND ADDITIVES Clays Sand Properties • • • • • • • • • • • • • • Green Compression Strength Dry Compression Strength Hot Compression Strength Moisture (water) Permeability Flowability Refractoriness Thermal Stability Collapsibility Produces good casting finish Mold Hardness Deformation Is reusable Remove heat from the cooling casting GENERAL PROPERTIES OF MOLDING SANDS • From a general viewpoint, the molding sand must be readily moldable and produce defect‐free castings if it is to qualify as a good one. Certain specific properties have been identified, and testing procedures adapted for their quantitative description. • The AFS "Foundry Sand Hand‐book"1 sets forth the standard conditions of testing the sand properties. Those properties of most obvious importance include: GENERAL PROPERTIES OF MOLDING SANDS 1. Green strength. The green sand, after water has been mixed into it, must have adequate strength and plasticity for making and handling of the mold. 2. Dry strength. As a casting is poured, sand adjacent to the hot metal quickly loses its water as steam. The dry sand must have strength to resist erosion, and also the metallostatic pressure of the molten metal, or else the mold may enlarge. GENERAL PROPERTIES OF MOLDING SANDS 3. Hot strength. After the moisture has evaporated, the sand may be required to possess strength at some elevated temperature, above 100 oC. Metallostatic pressure of the liquid‐metal bearing against the mold walls may cause mold enlargement, or if the metal is still flowing, erosion, cracks, or breakage may occur unless the sand possesses adequate hot strength. 4. Permeability. Heat from the casting causes a green‐sand mold to evolve a great deal of steam and other gases. The mold must be permeable, i.e. porous, to permit the gases to pass off, or the casting will contain gas holes. GENERAL PROPERTIES OF MOLDING SANDS 5. Thermal stability. Heat from the casting causes rapid expansion of the sand surface at the mold‐ metal interface. The mold surface may then crack, buckle, or flake off (scab) unless the molding sand is relatively stable dimensionally under rapid heating. 6. Refractoriness. Higher pouring temperatures, such as those for ferrous alloys at 2400 to 3200 F, require greater refractoriness of the sand. Low‐ pouring‐temperature metals, for example, aluminum, poured at 1300 F, do not require a high degree of refractoriness from the sand. GENERAL PROPERTIES OF MOLDING SANDS 7. Flowability. The sand should respond to molding processes. 8. Produces good casting finish. 9. Collapsibility. Heated sand which becomes hard and rocklike is difficult to remove from the casting and may cause the contracting metal to tear or crack. 10. Is reusable. 11. Offers ease of sand preparation and control. 12. Removes heat from the cooling casting. This list by no means includes all the properties which might be desirable. Obviously, the most important characteristic of a molding sand is that it facilitate the economic production of good castings. Sand Tests Generally the following tests are performed to judge the molding and casting characteristics of foundry sands: 1. Moisture content Test 2. Clay content Test 3. Chemical composition of sand 4. Grain shape and surface texture of sand. 5. Grain size distribution of sand 6. Refractoriness of sand 7. Strength Test 8. Permeability Test 9. Flowability Test 10. Shatter index Test 11. Mould hardness Test 28 Compiled by Prof. Amruta A. Rane (Asst. Prof., DJSCE) SAND ADDITIVES • • • • • • • Clays Water Carbons Cellulose Oil‐Chemicals Refrakteries Starches‐Solubles (Nişaşta) SAND ADDITIVES Clays • • • • • Clays Bentonite, Southern (Ca‐Bentonite) Bentonite, Western (Na‐Bentonite) Fireclay Kaolin Clay SAND ADDITIVES Clays SAND ADDITIVES Clays SAND ADDITIVES Clays SAND ADDITIVES Clays SAND ADDITIVES Water • Water • H0 2 SAND ADDITIVES Carbons • • • • • • • • Carbons Asphalt Gilsonite ( a kind of asphalt) Graphite Lamp Black (lamba isi) Lignite (brown coal) Pitch, Coal Tar (zift, kömür katranı) Seacoal (pulverized coal) • Carbon is added to the mold to provide a reducing atmosphere and a gas film during pouring that protects against oxidation of the metal and reduces burn‐in. • Carbon can be added in the form of seacoal (finely ground bituminous coal), asphalt, gilsonite (a naturally occurring asphaltite), or proprietary petroleum products. • Seacoal changes to coke at high temperatures expanding three times as it does so; this action fills voids at the mold/metal interface. Too much carbon in the mold gives smoke, fumes, and gas defects, and the use of asphalt products must be controlled closely because their overuse waterproofs the sand. • The addition of carbonaceous materials will give improved surface finish to castings. Best results are achieved with such materials as seacoal and pitch, which volatilize and deposit a pyrolytic (lustrous) carbon layer on sand at the casting surface.
© Copyright 2021 Paperzz